Injection Moulding Guidelines 1
Injection Moulding Guidelines
Injection Moulding Guidelines Injection Moulding Guidelines2 3
1. Introduction 3
2. Product overview 4
3. Machine selection and auxiliary equipment 5
4. Processing parameters 6
4.1. Drying 6
4.2. Setting temperatures 7
4.3. Screw speed and back pressure 8
4.4. Injection and holding phase 9
4.5. Cooling time 11
4.6. Cleaning the plasticizing unit 12
5. Troubleshooting 14
5.1. Moisture Streaks 16
5.2. Colour Streaks 17
5.3. Air Streaks 18
5.4. Burnt Streaks 19
5.5. Gloss variations 20
5.6. Weld lines 21
5.7. Sink marks 22
5.8. Jetting 23
5.9. Diesel effect 24
5.10. Stress cracks (whitening) 25
5.11. Flashes 26
5.12. Flaking 27
5.13. Cold flow lines 28
5.14. Dark sports 29
5.15. Trapped air in the injected parts 30
Table of contentsThis guide was prepared with the objective of helping injection moulders to run their projects smoothly without problems deriving in costly situations.
The guide is divided in two main parts related to the stage of the project: design and production. The first one will offer some clues for selecting the right equipment, tools and processing parameters in order to achieve a good performance in your injection projects when using ELIX materials. Different aspects like the selection of an appropriate injection machine, screw design, screw rotation speed, drying conditions, and processing parameters will be dealt with.
The second part will assist injection moulders during production to face some of the most common defects found. Each defect will be described with the signs needed to recognize it, the root causes of the defect and a procedure to solve the issue. Different possibilities will be contemplated in the troubleshooting procedures and they will be shown in the recommended order to follow. Only one parameter must be changed at a time in order to avoid interactions that may bring confusion about the correct path to solve the problem.
The procedures and hints contained in this guide are not intended to be followed literally but to serve as guidance. Selection of equipment, tools and processing parameters must be done case by case taking into account a great number of variables and no guide can contemplate all the possibilities. ELIX Polymers will not accept any responsibilities for the usage of this guide or any of the contents here contained. For more detailed information about any specific application, please contact our technical customer service.
Injection Moulding Guidelines Injection Moulding Guidelines4 5
ELIX Polymers, one of the main European engineering plastic players, started to act independently in October 2011, with a manufacturing capacity of 180kton/year and the experience of 40 years producing ABS and its blends at our plant in Tarragona (Spain).
State of the art technology, safe and environmentally responsible processes and an experienced sales & technical marketing team are the back-bone of our commitment to continuously bring value to our customers based all over the world.
ELIX Polymers products comprise a wide range of ABS products and derivates formulated for several processing techniques and different applications.
ELIX Polymers offers to their customers a wide range of injection moulding grades for several applications: general purpose, high heat, medical, food contact, electroplating, natural fibers, among others.
Every ELIX Polymer ABS grade can be prepared under a catalogue of more than 2.000 colors in addition to the several additive packages that fulfill our customer requirements.
2. Product overview
3. Machine selection and auxiliary equipmentSelecting the right machine size and the auxiliary equipment is not an easy task and several data must be known:
As ELIX provides all grades in a great range of colours, there is no need for the processor to use specific designs with mixing or shearing sections in the metering zone. Only in the case the processor needs to colour ELIX grades the presence of these sections may be desirable.
Screw diameter should be chosen on the basis of the shot weight (or volume) needed to fill the mould. Recommended metering stroke is between 1D and 3D (where D, is the screw diameter). Larger values will result into defects due to air entrapment and shorter values will lead to thermal degradation due to excessive residence times.
Other recommended screw design parameters are an L/D ratio between 20:1 and 23:1, a flight depth ratio
ELIX Polymers recommends the use of standard screw geometry where a feeding zone, a compression and a metering zone are present. Lengths of those zones should be kept in the following ranges:
Shot weight and volume
Mould mounting dimensions
Special conditions for specified quality requirements
Feeding zone (50% - 60%)
Compression zone (20% - 25%)
Metering zone (20% - 25%)
On all nozzles care should be taken to ensure a good fit between the diameter of the nozzle aperture and the diameter of the gate. Alignment of the sprue bush and nozzle aperture must be checked to avoid malfunctions.
In the case of using mineral filled or glass filled grades attention should be given to the abrasion protection in screws and barrels.
BEARING CHANNEL DEPTH PITCH HELIX ANGLE
3 PIECE FREE FLOW VALVEFLIGHT WIDTH
between 2:1 and 2,5:1 and a pitch of 1D. Variations from these parameters must be tested individually.
Residence time of ELIX materials should be kept between 4 and 6 minutes. Lower residence times could lead to insufficient melt formation while greater values will generate polymer degradation and loss of properties.
Open nozzles are recommended. Shut-off nozzles can be used in easy flow materials but attention must be paid to degradation issues related to excessive shear or residence time. All nozzles should be heated and controlled independently. Dead spots and/or flow divisions must be avoided in all cases with a proper design using flow engineering tools.
Injection Moulding Guidelines Injection Moulding Guidelines6 7
4. Processing parameters4.1 Drying
Content (% weight)
Drying Time (h)
Circulation Dryer(50% Fresh air)
Fresh Air Dryer(High speed)
Injection Moulding Guidelines Injection Moulding Guidelines8 9
4.3 Screw speed and back pressureTypical aspects to be taken into account when setting screw speed are achieving a correct polymer melting without overheating and minimizing cycle time. With these objectives in mind, ELIX recommends the following peripheral speeds (m/s) which can be later correlated to screw revolution units (min-1) depending on the screw diameter. Back pressures should be set in order to assure an appropriate melting of the polymer. Back pressure levels in the order of 100 - 150 bar (hydraulic pressure between 5 and 15 bar) should ensure complete melting of the material.
ELIX EASYFLOWING GRADES
(VP) (m/s)0.05 - 0.3 0.05 - 0.3 0.05 - 0.4
Screew diameter (mm)
Vp= 0.05 m/s
Vp= 0.2 m/s
Vp= 0.3 m/s
50 100 150
4.4 Injection and holding phaseInjection and holding pressures (also injection speed) will depend largely on the characteristics of the end product and must be high enough to achieve sufficient cavity pressure to enable a complete fill of the mould cavity, without sink marks. Those values must be low enough to avoid excessive shear in nozzle and mould in order to prevent material degradation. The pressure values can differ considerably for a given mould, depending on factors such as injection speed, melt temperature and nozzle geometry.
Injection speed should be set depending on the size and shape of the moulded part and should be as fast as possible. Injection pressure should be kept high enough in order to ensure that the pressure value does not drop below the required set point values during the entire cycle. An injection pressure drop at the end of injection will mean that injection pressure is too low or the set speed is too high.
Best results will be achieved if injection speed is set slow at the start of the injection process and sharply increased after. Implementing a speed profile can lead to a constant flow-front and therefore avoid flow engineering problems like entrapped air, weld lines, bubbles, tear drops, streaks, diesel effect, among others. Reduction of the injection speed directly prior to switchover can help to prevent a backflow of melt.
20 4 6 8 10 12 14 16 18 20
Cycle time (s)
START OF INJECTION
POLYMER REACHESPRESSURE SENSOR
Injection Moulding Guidelines Injection Moulding Guidelines10 11
Cavity pressure curve
In order to avoid overpacking of